Download presentation

Presentation is loading. Please wait.

Published byMaleah Carville Modified over 2 years ago

1
3.5 STRAIN ENERGY When material is deformed by external loading, energy is stored internally throughout its volume Internal energy is also referred to as strain energy Stress develops a force, F = σ A = σ (x y)

2
3.5 STRAIN ENERGY Strain-energy density is strain energy per unit volume of material u = ∆U ∆V σ 2 = If material behavior is linear elastic, Hooke’s law applies, u = σ 2 σ2 2E = ( )

3
3.5 STRAIN ENERGY Modulus of resilience When stress reaches proportional limit, strain-energy-energy density is called modulus of resilience ur = σpl pl 2 σpl2 2E = A material’s resilience represents its ability to absorb energy without any permanent damage

4
3.5 STRAIN ENERGY Modulus of toughness Modulus of toughness ut, indicates the strain-energy density of material before it fractures Shaded area under stress-strain diagram is the modulus of toughness Used for designing members that may be accidentally overloaded Higher ut is preferable as distortion is noticeable before failure

5
EXAMPLE 3.1 Tension test for a steel alloy results in the stress-strain diagram below. Calculate the modulus of elasticity and the yield strength based on a 0.2%.

6
EXAMPLE 3.1 (SOLN) Modulus of elasticity Calculate the slope of initial straight-line portion of the graph. Use magnified curve and scale shown in light blue, line extends from O to A, with coordinates ( mm, 345 MPa) E = 345 MPa mm/mm = 215 GPa

7
EXAMPLE 3.1 (SOLN) Yield strength At 0.2% strain, extrapolate line (dashed) parallel to OA till it intersects stress-strain curve at A’ σYS = 469 MPa

8
EXAMPLE 3.1 (SOLN) Ultimate stress Defined at peak of graph, point B, σu = MPa

9
EXAMPLE 3.1 (SOLN) Fracture stress When specimen strained to maximum of f = 0.23 mm/mm, fractures occur at C. Thus, σf = 621 MPa

10
3.6 POISSON’S RATIO When body subjected to axial tensile force, it elongates and contracts laterally Similarly, it will contract and its sides expand laterally when subjected to an axial compressive force

11
3.6 POISSON’S RATIO Strains of the bar are: long = δ L lat = δ’ r Early 1800s, S.D. Poisson realized that within elastic range, ration of the two strains is a constant value, since both are proportional. Poisson’s ratio, ν = − lat long

12
3.6 POISSON’S RATIO ν is unique for homogenous and isotropic material Why negative sign? Longitudinal elongation cause lateral contraction (-ve strain) and vice versa Lateral strain is the same in all lateral (radial) directions Poisson’s ratio is dimensionless, 0 ≤ ν ≤ 0.5

13
EXAMPLE 3.4 Bar is made of A-36 steel and behaves elastically. Determine change in its length and change in dimensions of its cross section after load is applied.

14
EXAMPLE 3.4 (SOLN) Normal stress in the bar is σz = P A = 16.0(106) Pa From tables, Est = 200 GPa, strain in z-direction is z = σz Est = 80(10−6) mm/mm Axial elongation of the bar is, δz = zLz = [80(10−6)](1.5 m) = −25.6 μm/m

15
EXAMPLE 3.4 (SOLN) Using νst = 0.32, contraction strains in both x and y directions are x = y = −νstz = −0.32[80(10−6)] = −25.6 μm/m Thus changes in dimensions of cross-section are δx = xLx = −[25.6(10−6)](0.1 m) = −25.6 μm δy = yLy = −[25.6(10−6)](0.05 m) = −1.28 μm

16
**3.6 SHEAR STRESS-STRAIN DIAGRAM**

Use thin-tube specimens and subject it to torsional loading Record measurements of applied torque and resulting angle of twist

17
**3.6 SHEAR STRESS-STRAIN DIAGRAM**

Material will exhibit linear-elastic behavior till its proportional limit, τpl Strain-hardening continues till it reaches ultimate shear stress, τu Material loses shear strength till it fractures, at stress of τf

18
**3.6 SHEAR STRESS-STRAIN DIAGRAM**

Hooke’s law for shear τ = Gγ G is shear modulus of elasticity or modulus of rigidity G can be measured as slope of line on τ-γ diagram, G = τpl/ γpl The three material constants E, ν, and G is related by G = E 2(1 + ν)

19
EXAMPLE 3.5 Specimen of titanium alloy tested in torsion & shear stress-strain diagram shown below. Determine shear modulus G, proportional limit, and ultimate shear stress. Also, determine the maximum distance d that the top of the block shown, could be displaced horizontally if material behaves elastically when acted upon by V. Find magnitude of V necessary to cause this displacement.

20
EXAMPLE 3.5 (SOLN) Shear modulus Obtained from the slope of the straight-line portion OA of the τ-γ diagram. Coordinates of A are (0.008 rad, 360 MPa) G = = 45(103) MPa 360 MPa 0.008 rad

21
EXAMPLE 3.5 (SOLN) Proportional limit By inspection, graph ceases to be linear at point A, thus, τpl = 360 MPa Ultimate stress From graph, τu = 504 MPa

22
EXAMPLE 3.5 (SOLN) Maximum elastic displacement and shear force By inspection, graph ceases to be linear at point A, thus, tan (0.008 rad) ≈ rad = d 50 mm d = 0.4 mm τavg = V A 360 MPa = V (75 mm)(100 mm) V = 2700 kN

23
***3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE**

Occurs when material supports a load for very long period of time, and continues to deform until a sudden fracture or usefulness is impaired Is only considered when metals and ceramics are used for structural members or mechanical parts subjected to high temperatures Other materials (such as polymers & composites) are also affected by creep without influence of temperature

24
***3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE**

Stress and/or temperature significantly affects the rate of creep of a material Creep strength represents the highest initial stress the material can withstand during given time without causing specified creep strain Simple method to determine creep strength Test several specimens simultaneously At constant temperature, but Each specimen subjected to different axial stress

25
***3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE**

Simple method to determine creep strength Measure time taken to produce allowable strain or rupture strain for each specimen Plot stress vs. strain Creep strength inversely proportional to temperature and applied stresses

26
***3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE**

Defined as a metal subjected to repeated cycles of stress and strain, breaking down structurally, before fracturing Needs to be accounted for in design of connecting rods (e.g. steam/gas turbine blades, connections/supports for bridges, railroad wheels/axles and parts subjected to cyclic loading) Fatigue occurs at a stress lesser than the material’s yield stress

27
***3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE**

Also referred to as the endurance or fatigue limit Method to get value of fatigue Subject series of specimens to specified stress and cycled to failure Plot stress (S) against number of cycles-to-failure N (S-N diagram) on logarithmic scale

28
CHAPTER REVIEW Tension test is the most important test for determining material strengths. Results of normal stress and normal strain can then be plotted. Many engineering materials behave in a linear-elastic manner, where stress is proportional to strain, defined by Hooke’s law, σ = E. E is the modulus of elasticity, and is measured from slope of a stress-strain diagram When material stressed beyond yield point, permanent deformation will occur.

29
CHAPTER REVIEW Strain hardening causes further yielding of material with increasing stress At ultimate stress, localized region on specimen begin to constrict, and starts “necking”. Fracture occurs. Ductile materials exhibit both plastic and elastic behavior. Ductility specified by permanent elongation to failure or by the permanent reduction in cross-sectional area Brittle materials exhibit little or no yielding before failure

30
CHAPTER REVIEW Yield point for material can be increased by strain hardening, by applying load great enough to cause increase in stress causing yielding, then releasing the load. The larger stress produced becomes the new yield point for the material Deformations of material under load causes strain energy to be stored. Strain energy per unit volume/strain energy density is equivalent to area under stress-strain curve.

31
CHAPTER REVIEW The area up to the yield point of stress-strain diagram is referred to as the modulus of resilience The entire area under the stress-strain diagram is referred to as the modulus of toughness Poisson’s ratio (ν), a dimensionless property that measures the lateral strain to the longitudinal strain [0 ≤ ν ≤ 0.5] For shear stress vs. strain diagram: within elastic region, τ = Gγ, where G is the shearing modulus, found from the slope of the line within elastic region

32
CHAPTER REVIEW G can also be obtained from the relationship of G = E/[2(1+ ν)] When materials are in service for long periods of time, creep and fatigue are important. Creep is the time rate of deformation, which occurs at high stress and/or high temperature. Design the material not to exceed a predetermined stress called the creep strength

33
CHAPTER REVIEW Fatigue occur when material undergoes a large number of cycles of loading. Will cause micro-cracks to occur and lead to brittle failure. Stress in material must not exceed specified endurance or fatigue limit

Similar presentations

Presentation is loading. Please wait....

OK

EGM 5653 Advanced Mechanics of Materials

EGM 5653 Advanced Mechanics of Materials

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on tcp/ip protocol driver Ppt on biography of any english poet Ppt on material heritage of india Ppt on france in french language Ppt on energy giving foods Ppt on current account deficit and currency Ppt on different types of dance forms in africa Ppt on brain computer interface Ppt on mesoamerica and south america Ppt on bolivia water war